Nd:YAG Laser Beam Welding of Coated Steels Using a Modified
Nd:YAG Laser Beam Welding of Coated Steels
Using a Modified Lap Joint Geometry
Nd:YAG laser beam welding of galvanized and galvannealed sheet steels in the
lap-joint configuration is made possible using a modified joint geometry
BY M. P. GRAHAM, D. C. WECKMAN, H. W. KERR, AND D. M. HIRAK
ABSTRACT. The weldability of coated
sheet steels by Nd:YAG lasers has been
examined using a 250-W pulsed laser, a
1-kW pulsed laser and a 2-kW continuous wave (CW) laser. Seam welds were
produced in 0.75-mm-thick (23- gauge)
galvanized and galvannealed sheet steels
using a modified lap-joint configuration
consisting of a groove-shaped projection
in the top sheet of the joint. Experiments
were performed to assess the effects on
weld quality of coating type, groove-projection dimensions and laser process parameters.
Good quality welds, which failed at
levels comparable to the base metal in
shear tensile tests, were made over a
wide range of conditions using the CW
Nd:YAG laser, but could only be produced using a limited range of process
conditions with the two pulsed lasers.
Using the CW laser at a mean power of
1600 W, good quality welds could be
produced at speeds up to 60 mm/s (144
in./min). In comparison, the maximum
acceptable welding speed when using
the 250-W pulsed laser at 220 W laser
mean power was just 2.4 mm/s (5.4
in./min). The melting ratios of the welds
produced with the CW laser were found
to be about 0.25, while they were approximately 0.10 for the welds produced
using the pulsed lasers. Finally, the quality of welds produced was not affected by
the dimensions of the groove projection
or by the coating type.
M. R GRAHAM, D. C. WECKMAN, and H. W.
KERR, are with the Department of Mechanical
Engineering, University of Waterloo, Waterloo, Ontario, Canada. D. M. HIRAK is with Imperial Oil Resources. Ltd, Calgary, Alberta,
162-s I MAY 1996
The automotive industry uses zinc-rich
coated sheet steels extensively in auto
body components for enhanced corrosion
resistance. Laser beam welding is being
evaluated as an alternative joining technique for these sheet steels in the lap-joint
configuration, because it offers a number
of advantages over traditional resistance
spot welding practices. For example,
much less flange material is required for
laser welding, resulting in a potentially
significant weight reduction. As well, no
direct contact is required between the
welding machine and the workpiece and
access is only required from one side of
the weld joint. In addition, lasers, particularly Nd:YAG lasers whose output can be
transmitted through fiber-optic cables, can
be easily integrated into automotive robotic welding cells.
Laser beam welding of zinc-coated
sheet steel in the lap-joint configuration is
illustrated schematically in Fig. 1A. The
well-known problem with welding these
materials in this configuration is related to
the low boiling point of zinc
Laser Beam Welding
Galvanized Sheet Steels
Coated Sheet Steels
(906°C/1663°F) compared with the melting
(~1550°C/2822°F). During seam welding, the two zinc coatings at the interface
vaporize and expand rapidly when the
molten steel weld pool approaches the interface between the two steel sheets. With
no joint clearance between the sheets,
this vapor can only escape through the
molten weld pool, and this typically results in excessive weld porosity or complete expulsion of the weld metal.
Many different techniques have been
attempted to allow production of acceptable seam welds in the lap-joint configuration in coated sheet steels using both
CO 2 and Nd:YAG lasers and no joint
clearance between the two sheets of
steel. The use of CO 2 and Nd:YAG lasers
pulsed at different frequencies has been
reported to permit the production of
good quality, full joint penetration welds
with no joint clearance (Refs. 1-7). Unfortunately, acceptable welds have only
been created using a small window of
processing conditions and these conditions have been found to be affected by
a number of process parameters including the coating type and thickness, the
sheet thickness, the laser power and the
type of laser. The effects of pulsing of the
beam on the welding process are not yet
In a recent study, the weldability of
laser beam welding coated sheet steels in
a lap-joint configuration with no clearance between the sheets was examined
using a 2-kW Nd:YAG laser capable of
CW and sine or square wave modulated
output (Ref. 8). The results of the study
showed that good quality welds could
not be produced using these lasers when
there was no joint clearance between the
two sheets of steel. Invariably, the welds
displayed excessive porosity or complete
weld metal expulsion due to the zinc
vapor created at the interface between
the two sheets during welding.
Good quality laser beam seam welds
have been reported when the zinc coating in the area of the weld was removed
prior to welding (Refs. 9, 10); however,
the cost of this additional processing step
may be prohibitive. Alternatively, there
are a large number of laser welding techniques for laser beam welding of these
coated sheet steels which have been designed to provide adequate venting of the
zinc vapor from between the two sheets
rather than through the weld pool. Good
quality welds have been produced using
continuous wave (CW) CO 2 lasers and
both pulsed and CW Nd:YAG lasers, for
example, by introducing a small joint
clearance between the sheets using preplaced shims as shown in Fig. 1 B (Refs.
11-13). It has been shown that clearances
ranging from 0.04 to 0.3 mm (0.0016 to
0.01 in.), depending on the type of coating, coating thickness, etc., provide an alternate path for venting of the zinc vapor
(Refs. 8, 12-15). For a particular coated
sheet steel, however, good quality welds
can only be produced over a narrow
range of clearance sizes (on the order of
0.1 to 0.2 mm/0.004 to 0.008 in.) and the
required joint clearance depends on a
number of variables including coating
type and thickness, sheet thickness, laser
type and beam diameter, and welding
speed. Although this approach has been
shown to permit the production of good
quality laser beam welds in a laboratory
setting, the difficulty of maintaining a
controlled joint clearance between the
sheets has prevented rapid acceptance of
a fixed-clearance technique in production environments.
Coated sheet steels have been laser
welded using a number of modified lapjoint geometries, which have been designed to create a controlled joint clearance between the sheets with minimal
fixturing. This has been done dynamically during welding using a roller device
(Ref. 16) or by prestamping stand-off projections into the top steel sheet and welding through the clearance between the
projections as shown in Fig. 1C (Refs.
17-19). The difficulty with these techniques remains that the required joint
clearance is still within a narrow range of
dimensions and is sensitive to variations
of many of the process parameters, as described above.
In the present study, a new joint
geometry for laser welding of these
coated materials in a lap-joint configuration was developed and evaluated. The
geometry consists of a rounded grooveshaped projection pressed into the top
sheet of the lap-joint specimen pair, as
shown in Fig. 2. This
technique differs from
the previously reported
preformed projections as
described above in that
the weld is made along
the point of contact between the two sheets
rather than through the
clearance created by the
projection. The advantage of this new joint
geometry is that it allows
the top and bottom
sheets to be clamped
firmly in contact during
welding while still providing a vent path between the sheets for the
zinc vapor to dissipate. It
has the additional advantages that weld quality is
not sensitive to dimensional variations of the
joint clearance formed
between the sheets and
that the groove can be
followed easily by a realtime joint tracker.
The objective of the
work reported here was
to evaluate the weldability of galvanized and galvannealed sheet steels
with the grooved-projection lap-joint configuration using three Nd:YAG
lasers; a 250-W pulsed
laser, a 1-kW pulsed laser
and a 2-kW CW laser.
The specific aims were to
determine the possible
influences on weld
quality of various
process parameters including output power
waveform, mean laser
power, welding speed,
geometry and coating
.L,c, 9 POOL
Fig. I - - Schematic diagrams of weld joint geometries previously
proposed for laser beam seam welding of coated sheet steels: A
- - No joint clearance between the sheets; B - - a defined joint
clearance between the sheets; C - defined joint clearances determined by prestamped projections in the top sheet.
Fig. 2 - - Schematic diagram of the groove-projection joint geometry used in this study for Nd:YAG laser beam seam welding of
coated sheet steels.
coated sheet steels
were used in this
galvanized sheet with a
minimum zinc coating of
60 g/m 2 on each side
(nominal coating thick-
Fig. 3 - - The clamping arrangement used for holding the weld
specimens and the gas cup assembly of the JK702 pulsed Nd:
WELDING RESEARCH SUPPLEMENT I 163-s
prototype MW2000 CW
laser and the JK706
pulsed laser were transmitted to the workpiece
0.8through a 25- and 15-m
long (82- and 49-ft), 1000Z
cable, respectively. Each
beam was then recolliuJ
mated by a lens as it ex0.4ited the fiber and focused
with a final process lens.
nThe lens combinations for
0.2the MW2000 and JK706
lasers were: 160 and 80
mm; and 160 and 160
When using each
R A D I A L P O S I T I O N (urn)
laser, a preliminary set of
welds was made to idenFig. 4 - - Representative power density distribution measured tify the optimum position
using a laser beam analyzer (LBA) at the focal position used in
of the beam focus relative
the experiments of the JK706 Nd:YAG laser when operating at to the groove surface on
600-W output power and with a 160/160-mm lens combination.
the basis of maximum
penetration for a given
laser power. This optiness -8 tim), and 0.79-mm (0.03-in.)
mum position was different for each mathick galvannealed sheet with a minichine and is listed in Table 3. A laser
mum coating of 40 g/m 2 (nominal coatbeam analyzer (LBA) (Ref. 20) was used
ing thickness 6 lam). The compositions of
then to measure the spatial distribution of
the steel substrates are shown in Table 1.
power density and the I/e2 diameter of
The laser welding experiments were
the laser beam at this operating position
conducted using either 25 x 50-mm or 50
in the laser beam. The measured beams
x 150-mm (1 x 2-in. or 2 x 6-in.) coupons
were multimode, but could be described
approximately by a Gaussian distribuof the coated sheet steels. To examine the
tion, as shown in Fig. 4. The I/e2 beam dieffects on weld quality of the groove proameters at the groove surface are listed
jection dimensions, grooves were
also in Table 3.
pressed a predetermined depth into the
In some welding trials using the protop sheet of a specimen pair using either
totype MW2000 laser and all of the weld0.99 or 1.40 mm (0.038 or 0.055 in.) diing trials performed with the JK702, the
ameter piano wires. The dimensions of
beam delivery system remained stationthe groove projections used in this study
ary and an x-y positioning table was used
are listed in Table 2. Prior to welding, all
to move the workpiece at the desired
specimens were ultrasonically cleaned
rate. In other trials with the MW2000
in varsol and dipped in N-Heptane to relaser and all experiments performed with
move dirt and oil. The two coupons of
the JK706 laser, the specimen to be
sheet steel were then clamped using the
welded was stationary and the fiber-optic
weld jig shown in Fig. 3 such that they
beam delivery head was moved over the
were in contact only along the projection
weld specimen using a Fanuc robot.
and welded along their line of contact as
In the first and second series of experillustrated in Fig. 2.
iments, the JK702 and JK706 pulsed
The laser welding machines used for
lasers were used to explore the effects on
this study were a 250-W pulsed Nd:YAG
weld quality of laser mean power, peak
laser (JK702), a 1-kW pulsed Nd:YAG
power and welding speed, and hence the
laser (JK706), and a prototype 2-kW CW
amount of pulse overlap, when welding
Nd:YAG laser (MW2000), all manufacgalvanized sheet steel with the series A
tured by Lumonics Corp. The JK702
groove-projection joint geometry-Table
pulsed laser had an adjustable beam ex2. In the first series of experiments with
panding telescope (BET) and a 120-mm
the JK702 laser, welds were made using
final focusing lens. The laser beams of the
Table 1 - - Composition (wt-%) of the 23-Ga Steel Sheet Substrates
164-sl MAY 1996
a laser mean power of 220 W. This mean
power was kept constant in order to prevent variation of the beam mode and diameter due to thermal lensing effects
(Ref. 21). Various combinations of pulse
energy and pulse time were obtained
while using this constant mean power by
varying the pulse frequency. For a particular welding condition (mean power,
pulse energy, pulse time and frequency)
the percentage of overlap between the
pulse varied with welding speed. About
20 welds were made using an orthogonal
matrix of experimental conditions in
order to identify the pulse conditions that
could be used to produce full penetration
welds. The welding speeds used were
2.4, 3.6 and 4.8 mm/s, (5.6, 8.5 and 11.3
in/min) and pulse energies were varied
from 31.9 to 38.3 J/pulse. Throughout
these experiments, argon shielding was
provided coaxially at a rate of 0.4 L/s
(11.3 fig/h) through a 6-mm (0.24-in.) diameter orifice located 9 mm (0.35 in.)
above the laser beam focal position.
In the second series of experiments,
the JK706 pulsed laser with the fiberoptic delivery system was used to make
22 full joint penetration welds using a
mean laser power of 720 W and a range
of process conditions. The varied parameters included: energy/pulse, pulse
time, focal position and welding speed.
Argon shielding was provided through a
12.8-mm (0.5-in.) diameter back-jet located approximately 10 mm (0.04 in.)
above the laser beam focal position at an
inclined angle of 30 deg to the weld
In a third series of experiments, the
prototype MW2000 CW laser was used
to make about 30 welds under various
process conditions in order to examine
the weldability of the galvanized sheet
steel with the series A and B groove-projection geometries - - Table 2. Welding
was performed at three mean powers:
685, 1000, and 1350 W using three to
five welding speeds for each mean
power. At 685 W, the three welding
speeds were 5, 7.5 and 10 mm/s (11.8,
17.7 and 23.6 in./min); at 1000 W, the
five welding speeds ranged from 15-30
mm/s (35.4-70.8 in./min); while at 1350
W, the five welding speeds ranged from
25-45 mm/s (59-106 in./min). In all
Table 2 - - Dimensions of Groove-Projection
Geometries Used in This Study
cases, the welding speed was not increased further if incomplete joint penetration through the bottom sheet was observed. Argon shielding gas was provided
coaxially at a rate of 0.4 L/s through a
3.2-mm (0.13-in.) diameter orifice located 3.5 mm (0.14 in.) above the laser
beam focal position.
In the fourth series of experiments, the
prototype MW2000 CW laser was used
to explore the weldability of the galvanized and galvannealed sheet steel with
all four groove-projection geometries
listed in Table 2. Approximately 64 welds
were made at two laser mean powers,
1200 and 1600 W, and using four welding speeds for each mean power. At 1200
W, the four welding speeds ranged from
27 to 43 mm/s (63.7-101.6 in./min),
while at 1600 W, welding speeds ranged
from 40 to 60 mm/s (94.5-141.7 in./min),
where again, the welding speed was not
increased if there was incomplete penetration of the bottom sheet. Argon shielding was provided in the same manner as
described for the third series of experiments but was supplied at a rate of 0.23
L/s (6.5 ft3/h).
The weld bead geometry and weld
quality of the laser welds produced were
determined from transverse sections of
the welds. A section of each seam weld
was mounted in bakelite, then ground
and diamond polished. Macro-etching
was performed with a solution of picric
acid (4 g in 100 mL methanol). Weld dimensions were measured using a metalIographic microscope coupled to JAVA
image analysis software. Finally, the failure mode and the load to failure were investigated by performing transverse shear
Fig. 5 - - Weld produced in 23-ga galvanized sheet with series A groove-proje( tion ger~metry
using the JK702 pulsed laser at 220 W laser mean power with 34 J/pulse and a pulse time of 30
ms at 2.4 mm/s. A - - Top view; B transverse section.
Fig. 6 - - Weld produced in 23-ga galvanized sheet steel with series A groove-projection ge~;metry using the prototype MW2000 CW laser at a laser mean power of 1350 W and a welding
speed of 30 mm/s. A - - Top view; B - transverse section.
tensile tests on an Instron tensile testing
Results and Discussion
Good quality laser beam seam welds
were produced in galvanized specimens
with the series A groove-projection joint
geometry using all three lasers. The acceptable welds produced with the JK702
and JK706 pulsed lasers displayed
smooth top-bead surfaces with a fine rippled pattern generated by the successive
overlapping laser pulses (Fig. 5A);
whereas, the surface of the welds made
with the prototype MW2000 CW laser
displayed a centerline ridge running
along the weld - - Fig. 6A. As shown in
ENERGY / PULSE
WELDING SPEED (mm/s)
Fig. 7 - - Transverse shear load to failure vs. welding speed of the laser
beam welds produced in 23-ga galvanized sheet steel using groove-projection geometry A with the pulsed JK702 laser at a laser mean power of
ENERGY / PULSE
WELDING SPEED (ram/s)
Fig. 8 - - Transverse shear load to failure vs. welding speed of the laser
beam welds produced in 23-ga galvanized sheet steel using series A
groove-projection geometry with the pulsed JK706 laser at a laser
mean power of 760 W.
WELDING RESEARCH SUPPLEMENT I 165-s
z 250 •
.200 150 a.
< 100 o
W E L D I N G S P E E D (minis)
Fig. 9 - - Transverse shear load to failure vs. welding speed of the laser
beam welds produced in 23-ga galvanized sheet steel using series A
groove-projection geometry with the M W2000 CW laser.
Figs. 5B and 6B, cross-sections of satisfactory welds fabricated with the pulsed
and CW lasers were indistinguishable.
These sections are typical of the acceptable welds. They are keyhole-mode
welds that completely penetrate the second sheet of steel. There is no evidence
of porosity at the interface generated by
the vaporizing zinc layers, indicating that
this groove-projection joint geometry has
permitted adequate venting of the zinc
vapors between the two sheets of steel
Welds displaying acceptable surface
quality were made with the pulsed lasers
over a limited range of processing conditions. The window of operating conditions which produced acceptable welds
with the JK702 laser was concentrated at
the upper limit of the laser's capabilities.
Table 3 - - Optimum Location of the Laser
Focal Position during Welding for Each
Laser, and Resulting Laser Beam Diameter at
the Groove Surface
of the Focused
5.0 mm above
0.5 mm below
1.0 mm below
166-s I MAY 1996
Fig. 10 - - Tranverse section of a weld produced in 23-ga galvannealed sheet at 60
mm/s using 1600-W laser mean power and
the series C groove-projection geometry.
Note the porosity at the bottom of the groove
due to inadequate venting of zinc vapor.
Using the laser mean power of 220 W,
good quality welds were produced at
welding speeds ranging from 2.4 to 4.8
mm/s using laser pulse energies ranging
from 31.9 to 38.3 J and pulse durations
of 30 ms. The top surface of the welds
produced at the lowest welding speed of
2.4 mm/s displayed pulse-to-pulse overlaps of approximately 75%. The backside
of these welds showed continuous complete penetration or discontinuous penetration. The top surface of the welds produced at higher welding speeds
displayed a lower amount of pulse-topulse overlap, while the backsides of the
weld specimens generally did not show
complete joint penetration. Welds fabricated at lower energies/pulse displayed
inadequate penetration into the second
sheet, while welds made at shorter pulse
times suffered from blowholes, and in
some cases, significant material loss. The
tolerance box of acceptable processing
conditions for welds made using the
JK706 pulsed laser was centered about a
pulse energy of 14.4-22.4 J/pulse with
pulse times ranging from 2.5 to 2.8 ms.
As in the case of the welds produced by
the JK702 laser, the top surface of the
welds produced at the lowest welding
speed displayed a high percentage of
pulse-to-pulse overlapping, on the order
of 78 to 81%. The backside surface of
these welds showed either continuous
complete penetration or discontinuous
penetration. As the welding speed increased, the amount of pulse-to-pulse
overlap on the top surface decreased and
the backside penetration showed re-
Welds displaying good surface quality
were made with the prototype MW2000
CW laser over a large range of laser mean
powers and welding speeds. In general,
acceptable quality welds were produced
at laser mean powers of 1000 W or more
and at speeds in excess of 20 mm/s. Complete joint penetration welds were produced when using 1600 W at speeds up
to 47 mm/s, while partial joint penetratration welds were successfully made at
speeds up to 60 mm/s.
The results of transverse shear tensile
testing of the welds made using the
JK702, JK706, and prototype MW2000
lasers are shown in Figs. 7, 8 and 9, respectively. For welds produced using the
JK702 pulsed laser (Fig. 7), failure loads
comparable to the base metal were observed for welds produced using the
three highest energies/pulse and the lowest welding speed, 2.4 mm/s. Failure of
these welded specimens always occurred in the base metal, it may be seen
from this graph that the failure load per
unit distance at a particular welding
speed generally decreased with decreasing energy/pulse. The decrease in failure
load per unit length seen with declining
energies/pulse is also a consequence of
reduced penetration into the second
sheet. Also, the failure load decreased
rapidly with increasing welding speed.
Similarly, the decrease in failure load per
unit distance with increasing welding
speed can be attributed to reduced
amounts of penetration of the second
sheet due to lower amounts of pulse overlapping with increased welding speed.
Similar trends were seen in the data obtained from the welds produced with the
JK706 pulsed laser, as shown in Fig. 8.
Once again, high failure loads with failure
occurring in the base metal were associated with the highest energies/pulse at one
welding speed, which in this case was 11
mm/s. This welding speed is more than
four times greater than that possible with
the JK702 pulsed laser.
The shear tensile strengths of the
MW2000 CW laser welds are plotted vs.
welding speed in Fig. 9. The welds made
using laser mean powers of 1000 and
1350 W from the third series of experiments had failure loads comparable to
the base metal and failed in the base
metal. At the lowest laser mean power
used, 685 W, and consequently, the lowest welding speeds, poor failure loads per
unit distance were seen with failure occurring in the heat-affected zone or weld
metal. These welds were characterized
by wide top beads and poor penetration
into the second sheet due to poor coupling of the laser beam with the workpiece at this laser mean power.
The transverse tensile shear strength
and weld quality of all laser beam seam
welds were adversely affected by misalignment of the laser beam with the centerline of the groove projection. An example of a transverse section through
such a weld is shown in Fig. 10. In general, the surface quality of these welds
was good and the misalignment of the
laser beam on the surface of the workpiece was easily seen. However, this misalignment caused a reduction in the weld
Fig. 11 - - Views of the bottom surface of longitudinal welds produced in 23-ga galvanized sheet
using series A groove-projection geometry which failed at levels comparable to the base metal. A
- - Backside of specimen displayed a few isolated areas of complete joint penetration; B - - backside of specimen displaying continuous full joint penetration.
strength, and in most cases, a change in
failure mode from failure in the base material to failure along the weld interface.
Also, as may be seen in Fig. 10, misalignment of the laser beam sometimes
caused intermittent weld metal porosity
due to incomplete venting of the zinc
vapor at the contact point between the
bottom of the groove and the second
sheet. In the extreme weld metal sagging
or drop-through occurred, because the
weld was created on the shoulder of the
groove where the joint clearance was excessive. While experiments were not performed specifically to establish laser
beam misalignment tolerance bands for
successful welds with the groove geometry, examination of welds such as the
one shown in Fig. 10 suggests that good
welds should be produced provided the
beam is within one beam radius of the
groove centerline. For the weld in Fig.
10, which was produced using the
MW2000 laser welding machine, the tolerance band would be about + 350 pm
(Table 3). Thus, these defects can be
eliminated easily by minimizing laser
beam misalignment using careful jigging
or by using a joint tracker to follow the
groove during welding.
Generally, the failure load and failure
mode of welds that displayed acceptable
surface quality could be predicted based
on the degree of joint penetration evident
on the backside of the workpiece. The
shear tensile testing results indicated that
welds which failed at relatively low
strength levels, with failure occurring in
the heat-affected zone or weld metal,
showed varying degrees of heat marks
consisting of resolidified zinc, but no
areas of complete joint penetration on
the backside of the workpiece. The welds
which had some areas of complete joint
penetration on the backside of the workpiece, even a small amount, such as
shown in Fig. 11A, had failure loads comparable to the base metal, with failure occurring in the base metal. Failure also occurred in the base metal of welds which
displayed more complete penetration,
MEAN POWER (W)
Fig. 12 --Acceptable welding conditions for specimens with series
A groove-projection joint geometry for the three lasers used in this
study presented by welding speed vs. mean power.
Fig. 13 - - Melting ratio vs. welding speed of the laser beam welds
produced in 23-ga galvanized sheet steel with the series A grooveprojection geometry using the JK702 and JK706 pulsed lasers.
WELDING RESEARCH SUPPLEMENT I 167-s
for this combination
of material and laser
above which welds
can be expected to
become unacceptable due to the occurrence of humping
weld defects (Ref.
22). This limit was
not reached in the
'~ 100 O
WELDING SPEED (ram/s)
The conversion efficiency of electrical
energy to optical enFig. 14 - - Melting ratio vs. welding speed of the laser beam welds produced in 23-ga galvanized sheet steel with the series A groove-projec- ergy of most solidstate laser welding
tion geometry using the MW2000 CW laser.
machines is typically
less than 5%. Howsuch as shown in Fig. 11B.
ever, when considering the overall weldThe laser welding conditions resulting
ing process efficiency, it is usual to conin good quality welds that failed at levels
sider only the efficiency with which the
comparable to the base metal are plotted
output optical energy is used to form a
in Fig. 12 as a function of laser mean
fused joint. This effectiveness can be depower and welding speed. These condifined by either the melting efficiency or
tions were determined from a combinathe melting ratio (Refs. 23, 24). The melttion of qualitative evaluation of the weld
ing efficiency is defined as the ratio of ensurface quality and the shear tensile testergy required to heat and melt the weld
ing results. It can be seen from this graph
metal to the energy absorbed by the
that for each of the pulsed lasers acceptworkpiece; whereas, the melting ratio is
able quality welds were only produced at
defined as the ratio of energy required to
one welding speed. In contrast, good
heat and melt the weld metal compared
quality welds were fabricated over a
to the output of the heat source, in this
large range of conditions with the protocase, the measurable laser beam.
type MW2000 CW laser. While this
The melting efficiency of pulsed laser
graph indicates a trend toward higher alwelding processes is difficult to deterlowable welding speeds with increased
mine because accurate measurements of
available laser power, there will be a limit
the effective absorptivity are usually not
Fig. 15 - - Transverse sections of longitudinal welds produced in 23-ga galvanized sheet using the
MW2000 CW laser produced at a laser mean power of 1600 W at 40 mm/s with different series
groove-projection geometries. A - - Joint geometry D; B - - joint geometry A.
168-s L MAY 1996
possible. However, calculation of the
melting ratio is possible because it requires only measurements of the laser
beam energy and the volume of weld
metal. In this study, therefore, the melting
ratio was calculated for welds produced
with the three different lasers to assessthe
relative effectiveness of each laser. The
melting ratio, nmr, is defined as
V[ C (Tm -T0)+AHm]
where V is the melt volume (m3), p is density (kg/m3), Cp is the specific heat
(kJ/kg.K), Tmp is the melting temperature
(K), T o is the ambient temperature (K),
AH m is the latent heat of melting (kJ/kg)
and E is the energy (J) of the laser pulse or
beam. The thermophysical material
properties used were those for AIS11008
steel (Ref. 25).
Two different techniques were used to
calculate the melting ratios of individual
pulse welds vs. the melting ratios of a
train of overlapping pulses or CW welds.
For a single pulse weld, the volume of a
single pulse weld was determined by
measuring the boundary coordinates of
the weld cross-section using a metallographic image analysis technique. Assuming that the weld pool was axisymmetric in shape, these boundary
coordinates were then used to perform a
numerical integration to provide the volume of weld metal. This value and the
measured pulse energy used to produce
the weld pool were then substituted into
Equation 1 to calculate the melting ratio.
To determine the melting ratio for a
train of pulses or a CW seam weld, the
volume of weld metal produced per unit
time was calculated by multiplying the
welding speed by the cross-sectional
area of the weld as measured using the
metallographic image analysis technique. Assuming that the cross-sectional
weld profile remained constant along the
weld, this value for volume of weld metal
produced per unit time and the energy
input per unit time were used in Equation
1 to calculate the melting ratio.
The calculated melting ratios as a
function of welding speed are shown in
Figs. 13 and 14 for the pulsed lasers and
CW laser, respectively. From the graph of
results for the pulsed lasers (Fig. 13), it
can be seen that the individual pulse
melting ratios were as high as 0.4 and decreased with increasing welding speed
for each laser. It may be expected that the
melting ratio for the single pulse welds
would be constant and independent of
welding speed. The observed decrease of
the melting ratio with increased welding
speed may be due to an under estimation
of the actual weld pool volume for welds
<C 100 O
WELDING SPEED (mm/s)
Fig. 16 - - Transverse shear load to failure vs. welding speed of the laser
beam welds produced on 23-ga galvanized sheet steel using the four
different series o f groove-projection geometries studied with the
MW2000 CW laser at a mean power of 1600 W.
produced at the higher speeds. As the
welding speed increases, the weld pool
width will decrease and the weld pool
will become elongated in the direction of
welding. Weld volume calculations
based upon the weld cross-section and
the assumption of an axisymmetric weld
pool shape will, therefore, underestimate
the actual weld pool volume, thereby
causing a decrease in the calculated
melting ratio as was observed.
In Fig. 13, the melting ratios of welds
produced using pulse trains from both
pulse lasers were approximately 0.1 ; that
is, 10% of the laser beam energy actually
contributed toward melting of the metal.
Also, these values were always less than
the melting ratios of the individual pulse
welds at any given welding speed. This is
because seam welds are produced using
a pulsed laser by making a succession of
overlapping individual spot welds. Thus,
a portion of the weld metal is repeatedly
reheated and melted, which inherently
reduces the overall efficiency of the
process. As the welding speed increased,
the two types of melting ratios converged, because the amount of overlapping was reduced.
The melting ratios of welds produced
using the prototype MW2000 CW laser
are plotted as a function of welding speed
in Fig. 14. The melting ratios of the good
quality welds produced at 1000 and
1350 W from the third series of experiments had melting ratios of approximately 0.25 and did not vary significantly
with welding speed. This melting ratio is
150% greater than the melting ratios cal-
WELDING SPEED (mm/s)
Fig. 17 - - Transverse shear load to failure vs. welding speed of the laser
beam welds produced in 23-ga galvannealed sheet steel using the four
different series of groove-projection geometries studied with the
MW2000 CW laser at a laser mean power of 1600 W.
culated for the seam welds produced
using the pulsed lasers. However, these
melting ratios are still significantly less
than the maximum theoretical melting
efficiency of 48% for a CW complete
joint penetration weld derived by SwiftHook and Gick (Ref. 24). Finally, the
melting ratios of welds from the third series of experiments, which were produced at 685 W and previously deemed
unacceptable, had much lower melting
ratios which were comparable to the
melting ratios of trains of pulses from the
two pulsed lasers. This is consistent with
the previous observations of poor weld
quality and incomplete penetration in
welds produced using this lower power.
power of 1600 W are shown in Figs. 16
and 17, respectively. From these graphs,
it can be seen that all of the welds produced with both the galvanized and the
galvannealed specimens failed at levels
comparable to the base metal with failure occurring in the base metal. With the
galvanized material, no significant variation in strength was seen for the welds
produced with different groove sizes.
However, results from the galvannealed
specimens showed more variation of failure load per unit length as a function of
the groove sizes, especially at high welding speeds.
Effect of Groove Size and Coating Type
The weldability of coated sheet steels
when using a modified lap joint geometry consisting of a rounded grooveshaped projection pressed into the top
sheet of the specimen pair has been investigated by making seam welds using a
wide range of process conditions with
three different Nd:YAG lasers: a 250-W
pulsed laser, a 1-kW pulsed laser with a
fiber-optic delivery system and a prototype 2-kW CW laser with fiber-optic delivery system.
Good quality welds were produced in
0.75-mm-thick (23-gauge) galvanized
sheet steel with the two pulsed lasers
under a limited set of process conditions
and with the 2 kW CW laser over a wider
range of process conditions. The top surface features of the welds depended on
the output waveform (pulsed vs. CW),
but transverse sections of the good welds
Good quality welds were produced
with the prototype MW2000 CW laser in
both galvanized and galvannealed
welded specimens and with all four
groove-projection geometries used (see
Series A-D in Table 2). As illustrated by
the representative transverse sections of
welds produced using a large and a small
groove depth in Fig. 15, weld quality,
size and shape were not significantly affected by the variations in groove dimensions used in this study. The results
were also independent of coating type.
The results from the transverse shear
tensile tests of galvanized and galvannealed specimens made with the four different groove geometries from the fourth
series of experiments at a laser mean
WELDING RESEARCH SUPPLEMENT I 169-s
displayed no discernable differences.
The transverse shear tensile strength
of acceptable welds produced with all
three lasers was comparable to the base
metal strength. However, the strength of
the laser beam welds were adversely affected by laser beam misalignment with
the groove projection centerline, or incomplete penetration through the second sheet of steel.
The w e l d i n g speeds that produced
acceptable quality welds increased with
laser power. The fastest speeds that produced good quality welds in the 23-ga
coated sheet steels were 2.4 mm/s with
the 250-W pulsed laser, 11 mm/s with the
1 -kW pulsed laser and 60 mm/s with the
prototype 2-kW CW laser. The melting
ratios were approximately 0.1 in seam
welds produced using the pulsed lasers
but were about 0.25 in welds produced
using the CW laser. Thus, the overall
process efficiency was about 150%
greater when using a CW laser compared
to a pulsed laser. Finally, unlike previous
controlled joint clearance techniques,
weld quality of laser welds made with the
new groove-projection lap joint configuration was not found to be sensitive to the
groove dimensions, the type of coating or
variations in coating thickness.
This work was supported by the Ontario Center for Materials Research
(OCMR) and the Ford Motor Co. Lumonics Corp. graciously provided the use of
their high-power prototype Nd:YAG laser
facilities. The contributions of H. N.
Bransch formerly of Lumonics Corp. during the welding experiments and S. Hong
during metallurgical evaluation of the
laser welds are gratefully acknowledged.
1. Heyden, J., Nilsson, K., and Magnusson,
C. 1988. Laser welding of zinc coated steel.
Lasers in Manufacturing, ed. H. Hugel, pp.
93-104. Cotswold Press Ltd, Oxford, U.K.
2. Heyden, J., Nilsson, K., and Magnusson,
170-s I M A Y 1996
C. 1990. Laser welding of zinc coated steel.
The Industrial Laser Annual Handbook, 1990
Edition. Eds: D. Belforte and M. Levitt, pp.
161-167, Penn Well Books, Tulsa, Oka.
3. Kennedy, S. C., and Norris, I. M. 1989.
Nd:YAG laser welding of bare and galvanized
steels. Intl. Congress and Exposition, Detroit,
Mich., SAE Technical Paper 890887.
4. Berlinger, G., and Speranza, J. J. 1987.
Laser Welding Metal Sheets with Associated
Trapped Gases. U.S. Patent No. 4,684,779.
5. Washio, K. 1992. Welding and cutting of
car-body metal sheets with Nd:YAG lasers by
flexible fiber beam delivery. SheetMetal Welding Conf. V. AWS Detroit section. Detroit, Mich.
6. Aruga, S., Matsui, E., Okino, K., Takenaka, H., Sato, K., Kyusho, Y., and Washio, K.
1992. Efficient and high-quality overlap welding of car-body aluminum alloy and sheets
with high power Nd:YAG laser by flexible
beam delivery. Proc. Laser Advanced Materials Processing, LAMP '92, pp. 517-522. Nagaoka, Japan. Japan High Temperature Soc.
7. Washio, K., Takenaka, H., Okino, K.,
Aruga, S., Matsui, E., and Kyusho, Y. 1992.
Welding and cutting car-body metal sheets
with fiber delivered output from high-power
Nd:YAG lasers. NEC Research and Development, NEC Corp. 33 (1): 102-109.
8. Graham, M. P, Hirak, D. M., Kerr, H. W.,
Weckman, D. C. 1994. Nd:YAG laser welding
of coated sheet steels. Journal of Laser Applications.
9. Williams, S. W., Salter, P. L., Scott, G.,
and Harris, S. J. 1993. New welding process
for galvanized steel. Proc. 26th Intl. Syrup. Automotive Technology & Automation. Aachen,
Germany, pp. 49-56.
10. Pennington, E. J. 1987. Laser Welding
of Galvanized Steel. U.S. Patent No.
11. Rito, N., Ohta, M., Yamada, T., Gotoh,
J., and Kitagawa, T. 1988. Laser Welding
Method. U.S. Patent No. 4,745,257.
12. Aknter, R., Steen, W. M., and Cruciani,
D. 1988. Laser welding of zinc coated steel.
Lasers in Manufacturing, ed. H. Hugel, pp.
195-206. Cotswold Press Ltd., Oxford, U.K.
13. Akhter, R., and Steen, W. M. 1990. The
gap model for welding zinc coated steel sheet,
Proc. Intl. Conf. Laser Systems Application in
Industry. pp. 219-236. Assoc. Tecnica del'
14. Imhoff, R., Behler, K., Gatzweiler,
W.,and Beyer, E. 1988. Laser beam welding in
car body making. Lasersin Manufacturing. ed.
H. Hugel, pp. 247-258. Cotswold Press Ltd,
15. Bagger,C., Miyamoto, I., Olsen, F., and
Maruo, H. June, 1992. Process behaviour during high power CO 2 laser welding of zinc
coated steel. Proc. Laser Advanced Materials
Processing LAMP "92. eds. A. Matsunawa and
S. Katayama, pp. 553-558. Nagaoka, Japan.
Japan High Temperature Society.
16. Hanicke, L., and Strandberg, O. 1993.
Roof laser welding in series production. SAE
Intl. Congress and Exposition. Detroit, Mich,
SAE Technical Paper 930028.
17. Petrick, F. D. 1990. Method of Making
Hemmed Joints Utilizing Laser Welding. U.S.
Patent No. 4,916,284.
18. Piane, A. D., Sartorio, F., Cantello, M.
and Ghiringhello, G. 1987. Method of Laser
Welding Sheet Metal Protected by Low-Vaporizing-Temperature Materials. U.S. Patent
19. Spies, B., and Thoms, V. 1992. Welded
Lap or Web Joints for Galvanized Sheet. U.S.
Patent No. 5,104,032.
20. Hirak, D. M., Weckman D. C., and
Kerr, H. W. 1994, measuring the spatial intensity distribution of high power focussed laser
beam analyses, Meaure Sci & Techn;Vol. 5 pp
21. Bransch, H. N., Weckinan, D. C., and
Kerr, H. W. 1994. Effects of pulse shaping on
Nd:YAG spot welds in austenitic stainless
steel. Welding Journal 73(6): 141 -s to 151 -s.
22. Albright, C. E., and Chiang, S. 1988.
High-speed laser welding discontinuities.
Journal of Laser Applications 1(1): 18-24.
23. Fuerschbach, P. W. 1992. Melting efficiency in fusion welding. The Metal Science
of Joining. eds. M. J. Cieslak, J. H. Perepezko,
S. Kang, and M. E. Glicksman, pp. 21-29.
TMS-MME, Warendale, Pa.
24. Swift-Hook, D. T., and Gick, A. E. F.
1973. Penetration welding with lasers. Welding Journal 52 (11): 492-s to 499-s.
25. Pehlke, R. D., Jeyarajan, A., and Wada,
H. 1992. NTIS Report No. NSF-MEA-82028.
University of Michigan, Ann Arbor, Mich.